EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES

 Valentine Payne
 4 months ago
 Views:
Transcription
1 EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510
2 EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLY WOOD CONSIDERED AS ORTHOTROPIC MATERIALS 1 By Forest Products Laboratory, 2 Forest Service U. S. Department of Agiculture Abstract This is a mathematical analysis of the stress distribution existing near a hole in a wood or plywood plate subjected to tension, as, for example, near holes in the tension flanges of wood box beams. It is assumed that the strains are small and remain within the proportional. limit. In this analysis a large, rectangular, orthotropic plate with a small, elliptic hole at the center is subjected to a uniform tension along two opposite edger. By taking equal axes for the elliptic hole, the theoretical stress distribution in the neighborhood of a circular hole is obtained. The analysis shows that for a circular hole in a plainsawn plate of Sitka spruce a maximum tensile stress of 5.84S is attained, S being the uniform tension applied in the direction of the grain. This maximum stress occurs on the edge of the circular hole at the ends of the diameter parpendicular to the direction of the uniform tension. Although this stress concentration may be greater than that found in isotropic materials, it is much more sharply localized and is relieved by plastic flow when the stress exceeds the proportional limit. For the reader who does not wish to follow the mathematical details of this report, the formula for computing this maximum stress for wood or plywood and an explanation of the constants involved is given in the appendix. The formula has not 1 This progress report was originally preparted by the Forest Products Laboratory in Maintained at Madison, Wis., in cooperation with the University of Wisconsin. Report No AgricultureMadison
3 been confirmed by an extensive series of tests, but it was found to be in reasonably satisfactory agreement with the only test made. It is also demonstrated that for the Sitka spruce plate mentioned the maximum shear stress attained is 0.71S (fig. 5). The stress function from which these formulas for the orthotropic case are obtained is shown to reduce to the wellknown stress function for the isotropic case. Introduction An orthotropic material possesses three planes of elastic symmetry at right angles to each other. If from such a material a flat plate is cut parallel to a plane of symmetry, it will have two perpendicular axes of symmetry in the plane of the plate. In the discussion that follows, a large rectangular orthotropic plate of this type with its edges parallel to the axes of symmetry and with a small hole at its center will be considered. A uniform tension S will be taken to act on two opposite edges of the plate as shown in figure 1, and the resulting stress distribution will be obtained. Throughout the report it is assumed that the strains are small and remain within the limits of "perfect elasticity." The solution is first derived for an elliptic hole with major and minor axes coinciding with the axes of symmetry. By taking the major and minor axes equal, the solution for a circular hole is obtained. For the orthotropic plate, the solution for the circular hole is but slightly more simple than that for the elliptic hole. This is different from the corresponding problem for the isotropic plate. 3 The stressstrain distribution in the neighborhood of the circular hole is notably different in an orthotropic plate than in an isotropic plate as the concentration may be considerably higher and of a more localized character for the orthotropic than for the isotropic plate. Thus in a plate of plainsawn Sitka spruce with a uniform tension acting in the grain direction, the greatest stress component at the edge of the hole decreases rapidly to onehalf of its maximum value in a radial distance of less than onetenth of the radius. For the isotropic plate the corresponding stress component decreases to onehalf of its maximum value in a radial distance larger than onehalf of the radius from the edge of the hole. 3 Timoshenko, S. Theory of Elasticity. Report No
4 The Effect of Eliptic or Circular Holes on the Stress Distribution in a Wood Plate The components of stress and strain in a plate under plane stress are connected by the following relations 4 if the axes of x and y are taken as the axes of elastic symmetry of the orthotropic plate: (1) In these equations E x and E y are Young's moduli in the x and y directions, respectively. Poisson's ratio σ xy is the ratio of the contraction parallel to the y axis to the extension parallel to the x axis associated with a tension parallel. to the x axis and similarly for σ yx. The quantity µ xy is the modulus of rigidity associated with the directions of x and y. Since the equations of equilibrium are deduced with no reference to the law connecting stresses and strainns, they will be satisfied by a stress function F such that (2) 4 March, H.W., StressStrain Relations in Wood and Plywood Considered as Orthotropic Materials, U. S. Forest Products Laboratory Report No Report No
5 Substituting (2) in (1) and then making use of the compatibility equation the following differential equation, obtained: satisfied by the stress function F, is (3) In deriving (3), the relation 4 (4) has been used. It is convenient to rewrite equation (3) as 5 (5) where (6) by making the substitution (7) 5 March, H, W., Flat Plates of Plywood Under Uniform or Concentrated Loads, U. S. Forest Products Laboratory Report No Report No,
6 where (8) Substituting F = F(x + vη) in (5) leads to the following equation for v: (9) or Now let 6 (10) (11) then 6 For wood or plywood, k as defined here is probably always greater than 1. Report No
7 Hence, the roots of equation (9) are Equation (5) may now be written as (12) where (13) The solution of equation (13) is facilitated by taking F of the form (14) where (15) F o ( x, η ) is any particular solution of (12), and the letter R means that the real part of the expression in the bracket is to be taken. That (14) is a solution of (12) is easily established by direct substitution. Equations (12) and (14) hold for the stress function associated with any elastic problem of plane stress in an orthotropic plate with x and y axes chosen as described here. Report No
8 A suitable choice of F for the problem discussed is (16) where (17) (18) the boundary of the hole (fig. 1) is given by (19) and S is the uniform tension applied at the ends of the plate. In order that the stresses may be singlevalued, the square roots in (17) are to be chosen so that the following relations always hold: Report No
9 Then (20) and (21) On the boundary of the hole x and η are given by (19), so that (22) (23) Similarly, on the edge of the hole (24) Consider the boundary of the hole in figure 2, and orient the positive direction of the normal v and of the tangent τ relative to one another in a way similar to the orientation of the x and yaxis, respectively. Report No
10 Let X v ds and Y v ds represent and x  and y components of the force per unit thickness of the plate, acting on the element of arc ds of the boundary from the positive side indicated by the direction of positive v. Then But (25) so that (26) Report No
11 Equations (26) for a boundary on which no stresses act take the form Hence, and are constant along a free boundry. Then, on the boundary of the hole, (27) Substituting (23) and (24) in (20) and (21), it follows from (27) that and (28) Taking the real parts (29) These equations must be satisfied for any value of θ, hence Report No
12 and Therefore, (30) By using equations (30), the stress components are found to be (31) (32) (33) To obtain the stress components for a circular hole, it is only necessary to let b = a in equations (31), (32), and (33). Then Report No
13 (34) (35) (36) where (37) Expressions (31), (32), (33) are complicated and do not permit easy computation of the numerical values of the stresses. The most important information they contain is, of course, in the neighborhood of the hole. Stresses at the Edge of the Hole From equations (22), (23), and (24), it is found that over the edge of the elliptic hole Report No
14 (40) Since, by (15) αβ = 1, the real parts are given by (41) (42) (43) where (44) It is of interest to refer these stresses at the edge of the hole to a pair of axes at right angles to each other having the directions of the normal v and the tangent τ, respectively (fig. 2). In this coordinate system, the shearing stress and the tension (or compression) in the vdirection must vanish, as this is required by the boundary conditions. It is readily shown that T τ of equation (44) is the tension (or compression) in the tangential direction. The component of direct stress in the tangential direction is given by Report No
15 From (19) and (25), this becomes Substituting from (41), (42), and (43), the tangential stress is found to be identical with T t of equation (44). If ε 1, it follows that at the end of the axis perpendicular to the direction of the tension, that is for θ = 90 (fig. 1), T τ attains its maximum value, while at the end of the axis parallel to the tension, that is θ = 0, T τ attains its minimum value. Then (45a) (46) For an isotropic material, it follows from (6), (8), (11), and (15) that α = β = ε = 1. Introducing these values, (45a) and (46) become S( 2b + 1) a and S, respectively, as in the isotropic case. 3 Equation (45a) gives the tension at C (fig. 1) the highest stress occurring in the plate. Numerical values of this stress will be computed in the two cases b 1 a = 50 and b a = for a plainsawn plate of Sitka spruce whose 50 elastic moduli are given in table 1. The grain direction is taken parallel to the line θ = 0. When b = 50, the tension at C (fig. 1) is times the mean tension. a When b = 1, the tension at C (fig. 1) is times the mean tension. a 50 Report No
16 The ellipse when b a = 50 would appear as a straight crack perpendicular to the grain which might be approximated by a break in the fibers, such as a compression failure. A very small tension applied to the plate across the crack would set up a tension at the ends of very high intensity. If this high tension at the ends caused the crack to tear, the increase in length would exaggerate the stress still further, and the crack would continue to spread. When b = 1 the ellipse would appear as a straight crack running in the a 50 direction of the grain or of the tension. Such a crack does not produce great local stress, a conclusion which is almost selfevident. If the hole is circular ( b = 1), equations (41), (42), (43), and (44) reduce to a where The stress at the end of the diameter perpendicular to the direction of the tension for a circular hole is given by (45b) For an isotropic plate ( α = β = ε =1) this reduces to 3S, as is well known, 3 but for a wood plate, equation (45b) may give a stress as high as 5.84S (fig. 8). Report No
17 Experimental Verification of Maximum Stress This maximum stress was experimentally verified by compressing a quartersawn yellowpoplar board containing a circular hole. The dimensions of the board and hole and the position of the 1/8inch metalectric strain gages at P on the circumference of the hole and at Q at some distance from the hole are shown in figure 3. The gage measuring the maximum strain at P was placed inside the hole as shown in figure 3, since the maximum strain occurs just on the edge of the hole and dies off rapidly in the radial direction. The gage at Q is placed as far from the hole as is feasible for the specimen used. The gage length was assumed short enough to give a close approximation to the actual strain at the end of the diameter. Table 2 gives the experimental and the theoretical values of the strains at pints P and Q of figure 3. The theoretical strains were computed in terms of S from the stresses given by formulas (35) and (45b) using the elastic moduli of the yellowpoplar plate. These moduli were obtained from coupons cut from the specimen and are given in table 1. The experimental value of the ratio of the strain at P to the strain at Q (fig. 3) is about 16 percent less than the theoretical one. This difference is not considered serious as the mathematical analysis was based on the assumption that the dimensions of the plate were large as compared to the dimensions of the hole. Also the impossibility of measuring strain at a point acted to decrease the apparent ratio. It is important to note that the experimental ratio is considerably higher than the corresponding ratio existing for a circular hole in an isotropic plate. Shear Stress at the Edge of the Hole The expression (43) for the shear component at the edge of the hole is highly important when considering holes in wood plates. When the uniform tension is parrallel to the grain direction, this shear acts in the same direction, and its distribution may indicate where failure caused by shear will take place if the uniform tension is sufficiently high. This statement has experimental verification when b = 1, as this type of faila ure occurred in wood box beams with small circular holes in their tension flanges tested at the U. S. Forest Products Laboratory (see fig. 4), The failure occurred in the vicinity of the point of maximum shear, which occurs theoretically, as shown in figure 5, at about θ = 78. The shear stress at the edge of the hole was evaluated numerically when b a = 1 for a plainsawn plate of Sitka spruce whose elastic moduli are given in Report No
18 table 1. The results are given in table 3 for values of θ between 0 and 90 when the line θ = 0 is taken to be parallel to the grain of the wood. The shear at other points on the circle may be easily filled in from the given values. Figure 5 illustrates the variation of X y over the edge of the hole for spruce and an isotropic material. Stress Components at Points Along the x and yaxes Simple expressions will now be obtained for the stress components at points along the x and yaxes. Writing equation (31) as and performing similar operations on equation (32) and (33), it is found that (47) These equations can be reduced considerably when x = 0 or y = 0. The resulting equations then readily show how the stress concentration dies off with increasing distance from the hole. Report No
19 > For x = 0, y = a it follows that (48) > a and for y = 0, x = (49) When b a = 1 the distances from the center of the hole may be expressed as multiples of the radius by writing x 1 = x a, y 1 = y in equations (48) and (49). Hence, the a stress components at points along the positive yaxis for a circular hole are given by Report No
20 (50) and at points along the positive xaxis (51) Numerical values of the stress components X x and Y y at points along the x and y axis when b = 1 are given in tables 4 and 5 for a plainsawn plate of Sitka spruce. a The variation of these components is illustrated in figures 6, 7, 8, and 9, and the variation of the corresponding stress components for an isotropic material is also shown for comparison. It is evident from these figures that considerable differ ences may exist between the stress distribution developed in the orthotropic plate as compared to the isotropic plate. In particular, figure 8 shows that the maximum stress developed in the spruce plate is nearly twice the maximum stress developed in the isotropic plate. Report No
21 Displacements in the Neighborhood of a Circular Hole The expressions for the displacements in the neighborhood of a circular hole ( b = 1) will now be obtained. a Substituting (34) and (35) in the first two equations of (1), it is found that (52) Integration of equations (52), gives Report No
22 (53) These are the actual displacements except for the addition of a linear function of y and a linear function of x to the expressions for u and v, respectively. This is easily shown by deriving the expression for e xy = + and comparing it with the expression These additive functions may be made rotation about the origin. to vanish by fixing the origin and eliminating Next the real and imaginary parts of and of a similar expression for z 2 and w 2 will be found. TO do this, it will be useful to write Let (54) where Report No (55)
23 (56) Then (57) Similarly (58) where (59) (60) To keep the displacements singlevalued, Y 1 and Y 2 must always be taken so that the following relations hold: Report No
24 Taking the real parts, equations (53) become (61) (62) These equations for the displacements would be used to check data given by strain gages of finite length, since the strains computed from the gage readings are average strains. Isotropic Stress Function as the Limiting Case of the Orthotropic Stress Function It is of interest to obtain from (16) the stress function for the corresponding problem when b = 1 for an isotropic material. a Substituting from (15) and (30), (16) becomes Report No
25 (63) For an isotropic material φ becomes equal to 0, and α, β, and ε each becomes equal to unity as sh own by equations (6), (8), (11), and (15). For these values, parts of equation (63) take the indeterminate form 0 0. Evaluating by differentiating both numerator and denominator with respect to φ (remembering that z 1, x 2, γ 1, and γ 2 all contain φ ), It follows that Report No
26 Report No
27 Let φ = 0 and ε = 1. Then (64) takes the form (65) where On setting b = a, parts of equation (65) assume the indeterminate form 0. On evaluating (65), it is found that for the circular hole, 0 (66) (67) Since the constant 2a 2 log 2 will not appear in the stresses obtained from (67), it may be omitted. The real. part of (67) is in polar form: (68) Report No
28 which is the wellknown form for the stress function in the corresponding problem for the isotropic plate.3 The Effect of Elliptic or Circular Holes on_. the Stress Distribution in a Plywood Plate A plywood panel having the grain direction of each ply perpendicular to that of the adjacent plies and having a symmetrical construction may be considered as an orthotropic plate. The strains in such plywood may be obtained from the average stresses (to be defined later), or the average stresses from the strains, 4 by exactly the same relations as exist between the strains and stresses for an orthotropic plate if the apparent elastic moduli of the plywood are used as the elastic moduli of the orthotropic plate. The panel is assumed to remain flat under the application of the loading considered. The xaxis will be taken parallel to the grain direction of the face plies. The subscript 1 will be used to denote quantities associated with plies having grain direction parallel to the xaxis, and the subscript 2 will be used to denote quantities associated with plies having grain direction parallel to the yaxis. Let h 1 denote the total thickness of all plies having grain direction parallel. to the xaxis. Let h 2 denote the total thickness of all plies having grain direction parallel to the yaxis, For plies having grain direction parallel to the xaxis, the following relations hold (69) Report No
29 and for plies having grain direction parallel to the yaxis corrosponding equations hold if the subscripts are changed. Since the panel remains flat, it will be assumed that (e xx ) 1 = (e xx ) 2. (e yy ) 1 = (e yy ) 2, (e xy ) 1 = (e xy ) 2, and it is no longer necessary to write the strain components with subscripts. Solving equations (69) for the stress components gives (70) where Similar relations hold in the remaining plies if the subscripts are changed throughout. Assuming the plies are all rotary cut and from the choice of axes, the elastic constants have the following values in the respective plies: Report No
30 After making these changes, equations (70) become (71) where Report NO
31 It is now important to define the mean stress components X x and Y y by the following equations: (72) where h = h 1 + h 2, the overall thickness of the plywood, and the relation ham been used. Equations (72) may be rewritten as follows: (73) where (74) Report No
32 Solving equations (73) for the strain components gives or (75) where 7 (76) It is easily established that 7 Since σ xy, σ xy, etc. are usually small, E x and E y are approximately equal to E a and E b, respectively. Report No
33 In plies with grain direction parallel to the xaxis, the conditions of equilibrium require and similarly in the remaining plies Then (77) (78) and Report No
34 (79) (80) Adding equations (77) and (79) and dividing by h, it is found that (81) where, since in all plies the relation holds, the mean stress component X y is identical with the stress component X y. Similarly equation (78) and (80) yield (82) Equations (81) and (82) will be satisfied by a stress function F, such that (83) Substituting (83) in (75) and then making use of the compatibility equation Report No
35 the following differential equation satisfied by the stress function F is found: As in the treatment of equation (3), it will be convenient to rewrite this equation as (84) where (85) by making the substitution where (86) (87) The differential equations (84) and (5) are of the same form mathematically, and any solution of (5) is a solution of (84) if the appropriate constants are used. It is then possible by using equations (31), (32), and (33) to obtain the stress distribution in the neighborhood of an elliptic hole situated in the middle of a plywood plate subjected to a uniform tension, provided that the axes of the ellipse are parallel and perpendicular to the grain of the face plies and that the tension is applied parallel or perpendicular to the axes of the ellipse. Report No
36 Hence, if the K and ε calculated from the apparent clastic: moduli of plywood are used, all of the preceding discussion for orthotropic plates containing elliptic holes holds for plywood panels. Numerical values for the stresses at various points along the x and y axes in the case b = 1 for rotarycut Sitka spruce plywood having half a the material with grain direction parallel to the xaxis are given in tables 6 and 7. Figures 10, 11, 12, and 13 illustrate how these stresses vary in the neighborhood of the hole. The foregoing analysis for plywood is based on the assumption that all plies are rotary cut and of the same species of wood. When these assumptions are not fulfilled, it is easy to make suitable modifications in the analysis (see appendix). Report No
37 Appendix A plainsawn or a quartersawn wood plate ox a plywood plate may be considered to have two perpendicular axes of elastic symmetry in the plane of the plate. The discussion given in this appendix applies to a rectangular plate of this type with its edges parallel to the axes of symmetry and with a small circular hole at the center. The x and yaxes are taken as the axes of symmetry. A uniform tension S directed parallel to the xaxis is supposed to act on the two opposite edges of the plate, and the tensile stress on the edge of the hole at the end of the diameter perpendicular to the uniform tension is given by For wood, the constants that appear in this expression are defined a3 follows: ε α β e = natural logarithmic base E x = Young's modulus in the xdirection E y = Young's modulus in the ydirection µ xy = modulus of rigidity In the xyplane Report No
38 σ xy = the Poisson's ratio given by the ratio of the contraction parallel to the yaxis to the extension parallel to the x axis associated with a tension parallel to the xaxis. For plywood, equations similar to those already given for wood define ε, α, β, φ, and K if the remaining constants are as subsequently defined. The plies will be considered to be numbered consecutively from the upper to the lower face. The elastic moduli in the ith ply will be denoted by (E x ) i, (E y ) i, (µ xy ) i, and (σ xy ) i. The thickness of the ith ply is h i. That of the plate is h. Then approximately 4 The shear parallel or perpendicular to direction of the uniform tension and on the edge of the circular hole is given in the mathematical part of the report by equation (43) if b is set equal to a. By substituting the constants defined previously, this shear stress may be plotted as a function of the polar coordinate θ (fig. 5), and its maximum value read from the curve. Report No
39 Table 1. Elastic moduli of Sitka spruce and yellow popular 1 Species Sitka spruce Yellowpoplar 1 The elastic moduli of Sitka spruce are average values obtained from a large number of tests made at the U.S. Forest Products Laboratory. The elastic moduli of yellowpoplar are values obtained from the one specimen used in the experimental verification of this report. 2 Not used. Table 2. Observed and theoretical values of the strains at the points P and Q of figure 3 Type Strain at P Strain at Q Ratio of strain at P to strain at Q Observed Theoretical (computed from equations (35) and (45b)) Inch per inch Report No. 1510
40 Report No. 1510
41 Table 4. Values of the stress components at points along the xaxis exterior to a circle of radius a and with center at the origin for a plainsawn plate of Sitka spruce  Report No. 1510
42 Report No Table 5. Values of the stress components at points along the y axis exterior to a circle of radius a and with center at the origin for a plainsawn plate of Sitka spruce
43 Table 6. Values of the stress components at points along the xaxis exterior to a circle of radius a and with center at the origin for a rotarycut plywood plate of Sitka spruce Table values of the stress components at points along the yaxis exterior to a circle of radius a and with center at the origin for a rotarycut plywood plate of Sitka spruce Report No. 1510
44 Figure 1Elliptic hole in orthotropic plate. Figure 2.Orientationof positive normal and tangent on the boundary of the elliptic hole. Z M F
45 Figure 3.Circular hole in a quartersawn yellowpoplar board subjected to a uniform compression. Z M F
46 Figure 4.The tension flange of a loaded wood box beam showing shear failure caused by vertical holes. The beam is subjected to a lower load in A than in B. The small cracks occurred in the stresscoat, which was applied to the beam before testing. The small round objects paralleling the edge of the flange are Whittemore strain gage points. Z M F
47 Z M F Figure 6.Variation of the normal stress component χx at points along the xaxis exterior to a circular hole of radius a and with center at the origin for a plainsawn plate of Sitka spruce and for an isotropic plate.
48 Figure 7.Variation of the normal stress component Yy at points along the xaxis exterior to a circular hole of radius a and with center at the origin for a plainsawn plate of Sitka spruce and for an isotropic plate. ZM F
49 Figure 8.Variationof the normal stress component Xx at points along the yaxis exterior to a circular hole of radius a and with center at the origin for a plainsawn plate of Sitka spruce and for an isotropic plate. Z M F
50 Figure 9.Variation of the normal stress component Y y at points along the y axis exterior to a circular hole of radius a and with center at the origin for a plainsawn plate of Sitka spruce and for an isotropic plate. Z M F
51 Figure 11.Variation of the normal stress component Yy at points along the xaxis exterior to a cir cular hole of radius a and with center at the originfor a rotarycut plywood plate of Sitka spruce. Figure 10.Variation of the normal stress component Xx at points along the xaxis exterior to a circular hole of radius a with center at the origin for a rotarycut plywood plate of Sitka spruce Z M F
52 Figure 12.Variation of the normal stress component Xx at points along the yaxis exterior to a circular hole of radius a and with center at the origin for a rotarycut plywood plate of Sitka spruce. Figure 13.Variation of the normal stress component Yy at points along the yaxis exterior to a circular hole of radius a and with center at the origin for a rotarycut plywood plate of Sitka spruce. Z M F
DEFLECTION OF BEAMS WlTH SPECIAL REFERENCE TO SHEAR DEFORMATIONS
DEFLECTION OF BEAMS WlTH SPECIAL REFERENCE TO SHEAR DEFORMATIONS THE INFLUENCE OF THE FORM OF A WOODEN BEAM ON ITS STIFFNESS AND STRENGTHI (REPRINT FROM NATIONAL ADVISORY COMMITTEE FOR AERONAUTICS REPORT
More informationCORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS
CORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS By Edmond P. Saliklis 1 and Robert H. Falk ABSTRACT: The weakness of existing relationships correlating offaxis modulus of elasticity
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationMINIMUM WEIGHT STRUCTURAL SANDWICH
U.S. DEPARTMENT OF AGRICULTURE FOREST SERVICE FOREST PRODUCTS LABORATORY MADISON, WIS. In Cooperation with the University of Wisconsin U.S.D.A. FOREST SERVICE RESEARCH NOTE Revised NOVEMBER 1970 MINIMUM
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationCombined Stresses and Mohr s Circle. General Case of Combined Stresses. General Case of Combined Stresses con t. Twodimensional stress condition
Combined Stresses and Mohr s Circle Material in this lecture was taken from chapter 4 of General Case of Combined Stresses Twodimensional stress condition General Case of Combined Stresses con t The normal
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationS HEAR S TRENGTH IN P RINCIPAL P LANE OF W OOD
S HEAR S TRENGTH IN P RINCIPAL P LANE OF W OOD By Jen Y. Liu 1 and Lester H. Floeter 2 ABSTRACT: In this study, the writers used Tsai and Wu s tensor polynomial theory to rederive a formula originally
More informationFLEXURE OF STRUCTURAL SANDWICH CONSTRUCTION
FLEXURE OF STRUCTURAL SANDWICH CONSTRUCTION December 1951 INFORMATION REVIEWED AND REAFFIRMED 1958 LOAN COPY Please return to: Wood Engineering Research Forest Products Laboratory Madison, Wisconsin 53705
More informationPlane and axisymmetric models in Mentat & MARC. Tutorial with some Background
Plane and axisymmetric models in Mentat & MARC Tutorial with some Background Eindhoven University of Technology Department of Mechanical Engineering Piet J.G. Schreurs Lambèrt C.A. van Breemen March 6,
More informationEmpirical Prediction of Shear Modulus and Young's Modulus of Plywood Panels
Empirical Prediction of Shear Modulus and Young's Modulus of Plywood Panels By Edmond P. Saliklis Assistant Professor of Civil and Environmental Engineering 3 Alumni Hall of Engineering Lafayette College,
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationTHE BENDING STIFFNESSES OF CORRUGATED BOARD
AMDVol. 145/MDVol. 36, Mechanics of Cellulosic Materials ASME 1992 THE BENDING STIFFNESSES OF CORRUGATED BOARD S. Luo and J. C. Suhling Department of Mechanical Engineering Auburn University Auburn,
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationTHEORY OF PLATES AND SHELLS
THEORY OF PLATES AND SHELLS S. TIMOSHENKO Professor Emeritus of Engineering Mechanics Stanford University S. WOINOWSKYKRIEGER Professor of Engineering Mechanics Laval University SECOND EDITION MCGRAWHILL
More informationSTRESSEDSKIN PANEL DEFLECTIONS AND STRESSES USDA FOREST SERVICE RESEARCH PAPER
STRESSEDSKIN PANEL DEFLECTIONS AND STRESSES USDA FOREST SERVICE RESEARCH PAPER FPL 251 1975 U. S. DEPARTMENT OF AGRICULTURE FOREST SERVICE FOREST PRODUCTS LABORATORY MADISON, WISCONSIN ABSTRACT This paper
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationACCURATE FREE VIBRATION ANALYSIS OF POINT SUPPORTED MINDLIN PLATES BY THE SUPERPOSITION METHOD
Journal of Sound and Vibration (1999) 219(2), 265 277 Article No. jsvi.1998.1874, available online at http://www.idealibrary.com.on ACCURATE FREE VIBRATION ANALYSIS OF POINT SUPPORTED MINDLIN PLATES BY
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationBOOK OF COURSE WORKS ON STRENGTH OF MATERIALS FOR THE 2 ND YEAR STUDENTS OF THE UACEG
BOOK OF COURSE WORKS ON STRENGTH OF MATERIALS FOR THE ND YEAR STUDENTS OF THE UACEG Assoc.Prof. Dr. Svetlana LilkovaMarkova, Chief. Assist. Prof. Dimitar Lolov Sofia, 011 STRENGTH OF MATERIALS GENERAL
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More information6.1 Formulation of the basic equations of torsion of prismatic bars (St. Venant) Figure 6.1: Torsion of a prismatic bar
Module 6 Torsion Learning Objectives 6.1 Formulation of the basic equations of torsion of prismatic bars (St. Venant) Readings: Sadd 9.3, Timoshenko Chapter 11 e e 1 e 3 Figure 6.1: Torsion of a prismatic
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationCOMPRESSIVE EUCICLING CURVES MR SANDWICH PANELS WITH ISOTROPIC FACINGS AND ISOTROPIC OR ORTI1OTROIPIC CORES. No Revised January 1958
SRICULTU RE ROOM I COMPRESSIVE EUCICLING CURVES MR SANDWICH PANELS WITH ISOTROPIC FACINGS AND ISOTROPIC OR ORTI1OTROIPIC CORES No 1854 Revised January 1958 This Report is One of a Series Issued in Cooperation
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationBy drawing Mohr s circle, the stress transformation in 2D can be done graphically. + σ x σ y. cos 2θ + τ xy sin 2θ, (1) sin 2θ + τ xy cos 2θ.
Mohr s Circle By drawing Mohr s circle, the stress transformation in D can be done graphically. σ = σ x + σ y τ = σ x σ y + σ x σ y cos θ + τ xy sin θ, 1 sin θ + τ xy cos θ. Note that the angle of rotation,
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationLab Exercise #3: Torsion
Lab Exercise #3: Prelab assignment: Yes No Goals: 1. To evaluate the equations of angular displacement, shear stress, and shear strain for a shaft undergoing torsional stress. Principles: testing of round
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationTwodimensional ternary locally resonant phononic crystals with a comblike coating
Twodimensional ternary locally resonant phononic crystals with a comblike coating YanFeng Wang, YueSheng Wang,*, and Litian Wang Institute of Engineering Mechanics, Beijing Jiaotong University, Beijing,
More informationMachine Direction Strength Theory of Corrugated Fiberboard
Thomas J. Urbanik 1 Machine Direction Strength Theory of Corrugated Fiberboard REFERENCE: Urbanik.T.J., Machine Direction Strength Theory of Corrugated Fiberboard, Journal of Composites Technology & Research,
More information1 Stress and Strain. Introduction
1 Stress and Strain Introduction This book is concerned with the mechanical behavior of materials. The term mechanical behavior refers to the response of materials to forces. Under load, a material may
More informationUnit III Theory of columns. Dr.P.Venkateswara Rao, Associate Professor, Dept. of Civil Engg., SVCE, Sriperumbudir
Unit III Theory of columns 1 Unit III Theory of Columns References: Punmia B.C.,"Theory of Structures" (SMTS) Vol II, Laxmi Publishing Pvt Ltd, New Delhi 2004. Rattan.S.S., "Strength of Materials", Tata
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More informationACET 406 MidTerm Exam B
ACET 406 MidTerm Exam B SUBJECT: ACET 406, INSTRUCTOR: Dr Antonis Michael, DATE: 24/11/09 INSTRUCTIONS You are required to answer all of the following questions within the specified time (90 minutes).you
More informationMECH 401 Mechanical Design Applications
MECH 401 Mechanical Design Applications Dr. M. O Malley Master Notes Spring 008 Dr. D. M. McStravick Rice University Updates HW 1 due Thursday (11708) Last time Introduction Units Reliability engineering
More informationSpherical Pressure Vessels
Spherical Pressure Vessels Pressure vessels are closed structures containing liquids or gases under essure. Examples include tanks, pipes, essurized cabins, etc. Shell structures : When essure vessels
More informationBoundary Conditions in Fluid Mechanics
Boundary Conditions in Fluid Mechanics R. Shankar Subramanian Department of Chemical and Biomolecular Engineering Clarkson University The governing equations for the velocity and pressure fields are partial
More information(x 1, y 1 ) = (x 2, y 2 ) if and only if x 1 = x 2 and y 1 = y 2.
1. Complex numbers A complex number z is defined as an ordered pair z = (x, y), where x and y are a pair of real numbers. In usual notation, we write z = x + iy, where i is a symbol. The operations of
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationUniaxial Loading: Design for Strength, Stiffness, and Stress Concentrations
Uniaxial Loading: Design for Strength, Stiffness, and Stress Concentrations Lisa Hatcher This overview of design concerning uniaxial loading is meant to supplement theoretical information presented in
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More information1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine Spring 2004 LABORATORY ASSIGNMENT NUMBER 6
1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine MIT Spring 2004 LABORATORY ASSIGNMENT NUMBER 6 COMPRESSION TESTING AND ANISOTROPY OF WOOD Purpose: Reading: During this laboratory
More informationStress transformation and Mohr s circle for stresses
Stress transformation and Mohr s circle for stresses 1.1 General State of stress Consider a certain body, subjected to external force. The force F is acting on the surface over an area da of the surface.
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationDegree Thesis Flexural Rigidity (D) in Beams. Author: Zious Karis. Instructor: Rene Herrmann
Degree Thesis Flexural Rigidity (D) in Beams Author: Zious Karis Instructor: Rene Herrmann Degree Thesis Materials Processing Technology 2017 DEGREE THESIS Arcada University of Applied Sciences, Helsinki,
More information1131UCIAING CIF RAG, MN, PLYWOOD CYLINDERS IN AXIAL COMPRESSION
1131UCIAING CIF RAG, MN, PLYWD CYLINDERS IN AXIAL CMPRESSIN I nieftnatiett IkavictuciLn4114cattirmyd March 1 &6 INFRMAIMN REV AND REAFFIRML 1962 No. 1322 LAN CPY Please return to: Wood Engineering Research
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationMIETIIODS OF CALCULATING THE STRENGTH AND MODULUS Of!ELASTICITY. OF PLYWOOD IN COMIPPESSION
MIETIIDS F CALCULATING TE STRENGT AND MDULUS f!elasticity. F PLYWD IN CMIPPESSIN Revised September 1955 INFRMATIN REVIEWED AN REAFFIRMED 196 No. 1315 UNITED STATES DEPARTMENT F AGRICULTURE FREST SERVICE
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More information4. SHAFTS. A shaft is an element used to transmit power and torque, and it can support
4. SHAFTS A shaft is an element used to transmit power and torque, and it can support reverse bending (fatigue). Most shafts have circular cross sections, either solid or tubular. The difference between
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationOptimum Fiber Distribution in Singlewall Corrugated Fiberboard
United States Department of Agriculture Forest Service Forest Products Laboratory Research Paper FPL 348 1979 Optimum Fiber Distribution in Singlewall Corrugated Fiberboard Abstract Determining optimum
More informationStress, Strain, Mohr s Circle
Stress, Strain, Mohr s Circle The fundamental quantities in solid mechanics are stresses and strains. In accordance with the continuum mechanics assumption, the molecular structure of materials is neglected
More informationQuestion 1. Ignore bottom surface. Solution: Design variables: X = (R, H) Objective function: maximize volume, πr 2 H OR Minimize, f(x) = πr 2 H
Question 1 (Problem 2.3 of rora s Introduction to Optimum Design): Design a beer mug, shown in fig, to hold as much beer as possible. The height and radius of the mug should be not more than 20 cm. The
More informationFIXED BEAMS IN BENDING
FIXED BEAMS IN BENDING INTRODUCTION Fixed or builtin beams are commonly used in building construction because they possess high rigidity in comparison to simply supported beams. When a simply supported
More informationChapter 13 ELASTIC PROPERTIES OF MATERIALS
Physics Including Human Applications 280 Chapter 13 ELASTIC PROPERTIES OF MATERIALS GOALS When you have mastered the contents of this chapter, you will be able to achieve the following goals: Definitions
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationARC 341 Structural Analysis II. Lecture 10: MM1.3 MM1.13
ARC241 Structural Analysis I Lecture 10: MM1.3 MM1.13 MM1.4) Analysis and Design MM1.5) Axial Loading; Normal Stress MM1.6) Shearing Stress MM1.7) Bearing Stress in Connections MM1.9) Method of Problem
More informationLecture 3: The Concept of Stress, Generalized Stresses and Equilibrium
Lecture 3: The Concept of Stress, Generalized Stresses and Equilibrium 3.1 Stress Tensor We start with the presentation of simple concepts in one and two dimensions before introducing a general concept
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationME 383S Bryant February 17, 2006 CONTACT. Mechanical interaction of bodies via surfaces
ME 383S Bryant February 17, 2006 CONTACT 1 Mechanical interaction of bodies via surfaces Surfaces must touch Forces press bodies together Size (area) of contact dependent on forces, materials, geometry,
More informationShear coupling effects on stress and strain distributions in wood subjected to transverse compression
Composites Science and Technology 67 (2007) 1362 1369 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech Shear coupling effects on stress and strain distributions in wood subjected to
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More information7. STRESS ANALYSIS AND STRESS PATHS
71 7. STRESS ANALYSIS AND STRESS PATHS 7.1 THE MOHR CIRCLE The discussions in Chapters and 5 were largely concerned with vertical stresses. A more detailed examination of soil behaviour requires a knowledge
More informationBUTT SPLICE HINGING. KEVIN COLE, PhD Senior Web Handling Development Engineer Optimation Technology Incorporated
BUTT SPLICE HINGING BY KEVIN COLE, PhD Senior Web Handling Development Engineer Optimation Technology Incorporated Introduction Splicing is a process used to join the tail of an expiring roll to the start
More informationREEXAMINATION OF YLINEN AND OTHER COLUMN EQUATIONS
REEXAMINATION OF YLINEN AND OTHER COLUMN EQUATIONS By John J. Zahn 1 ABSTRACT: In 1991, Ylinen s column equation was adopted for the design of wood columns in the United States. Ylinen originally derived
More informationMECHANICS OF MATERIALS. Prepared by Engr. John Paul Timola
MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationCode_Aster. Calculation algorithm of the densities of reinforcement
Titre : Algorithme de calcul des densités de ferraillage Date : 05/08/2013 Page : 1/11 Calculation algorithm of the densities of reinforcement Summary: One presents the calculation algorithm of the densities
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationCBE 6333, R. Levicky 1. Orthogonal Curvilinear Coordinates
CBE 6333, R. Levicky 1 Orthogonal Curvilinear Coordinates Introduction. Rectangular Cartesian coordinates are convenient when solving problems in which the geometry of a problem is well described by the
More informationLINEAR AND NONLINEAR SHELL THEORY. Contents
LINEAR AND NONLINEAR SHELL THEORY Contents Straindisplacement relations for nonlinear shell theory Approximate straindisplacement relations: Linear theory Small strain theory Small strains & moderate
More informationCivil Engineering Design (1) Analysis and Design of Slabs 2006/7
Civil Engineering Design (1) Analysis and Design of Slabs 006/7 Dr. Colin Caprani, Chartered Engineer 1 Contents 1. Elastic Methods... 3 1.1 Introduction... 3 1. Grillage Analysis... 4 1.3 Finite Element
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationReview of Strain Energy Methods and Introduction to Stiffness Matrix Methods of Structural Analysis
uke University epartment of Civil and Environmental Engineering CEE 42L. Matrix Structural Analysis Henri P. Gavin Fall, 22 Review of Strain Energy Methods and Introduction to Stiffness Matrix Methods
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationMECH 344/X Machine Element Design
1 MECH 344/X Machine Element Design Time: M 14:4517:30 Lecture 2 Contents of today's lecture Introduction to Static Stresses Axial, Shear and Torsional Loading Bending in Straight and Curved Beams Transverse
More informationCIVL4332 L1 Introduction to Finite Element Method
CIVL L Introduction to Finite Element Method CIVL L Introduction to Finite Element Method by Joe Gattas, Faris Albermani Introduction The FEM is a numerical technique for solving physical problems such
More informationSoil strength. the strength depends on the applied stress. water pressures are required
Soil Strength Soil strength u Soils are essentially frictional materials the strength depends on the applied stress u Strength is controlled by effective stresses water pressures are required u Soil strength
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 4 Pure Bending
EA 3702 echanics & aterials Science (echanics of aterials) Chapter 4 Pure Bending Pure Bending Ch 2 Aial Loading & Parallel Loading: uniform normal stress and shearing stress distribution Ch 3 Torsion:
More informationContact, Adhesion and Rupture of Elastic Solids
D. Maugis Contact, Adhesion and Rupture of Elastic Solids With 186 Figures Springer Contents г 1. Elements of Surface Physics 1 1.1 Introduction 1 1.2 Van der Waals Forces Between Molecules 3 1.2.1 The
More informationFinite element analysis of diagonal tension failure in RC beams
Finite element analysis of diagonal tension failure in RC beams T. Hasegawa Institute of Technology, Shimizu Corporation, Tokyo, Japan ABSTRACT: Finite element analysis of diagonal tension failure in a
More informationMeasurement of Dynamic Viscoelasticity of FullSize Wood Composite Panels Using a Vibration Testing Method
Measurement of Dynamic Viscoelasticity of FullSize Wood Composite Panels Using a Vibration Testing Method Cheng Guan, a Houjiang Zhang, a, * John F. Hunt, b Lujing Zhou a and Dan Feng a The dynamic viscoelasticity
More informationTensor Transformations and the Maximum Shear Stress. (Draft 1, 1/28/07)
Tensor Transformations and the Maximum Shear Stress (Draft 1, 1/28/07) Introduction The order of a tensor is the number of subscripts it has. For each subscript it is multiplied by a direction cosine array
More informationThe subject of this paper is the development of a design
The erformance and Design Checking of ChordAngle Legs in Joist Girders THEODORE V. GALAMBOS ABSTRACT The subject of this paper is the development of a design checking method for the capacity of the outstanding
More information